Survey

Document related concepts

Transcript

Progress In Electromagnetics Research, Vol. 137, 359–370, 2013 NEAR INFRARED FILTERING PROPERTIES IN PHOTONIC CRYSTAL CONTAINING EXTRINSIC AND DISPERSIVE SEMICONDUCTOR DEFECT Chi-Chung Liu1 and Chien-Jang Wu2, 1 Department * of Electro-Optics Engineering, University, Yunlin 632, Taiwan, R.O.C. National Formosa 2 Institute of Electro-Optical Science and Technology, National Taiwan Normal University, Taipei 116, Taiwan, R.O.C. Abstract—In this work, near infrared ﬁltering properties in a transmission narrowband ﬁlter are theoretically investigated. The ﬁlter is a defective photonic crystal of (LH)N D(HL)N , where N is the stack number, L is SiO2 , H is InP, and defect layer D is an extrinsic semiconductor of n-type silicon (n-Si). It is found that there are multiple transmission peaks within the photonic band gap (PBG) as the defect thickness increases. The ﬁltering position can be changed by varying the doping density in n-Si. That is, the peak (channel) wavelength is blued-shifted when the doping density increases. In the angle-dependent ﬁltering property, the channel wavelength is also blued-shifted as the angle of incidence increases for both TE and TM waves. These ﬁltering properties are of technical use in the applications of semiconductor optoelectronics. 1. INTRODUCTION Photonic crystals (PCs) are periodic layered structures and can be classiﬁed as one-, two-, or three-dimensional. PCs can possess frequency regions in which the propagation of electromagnetic waves is forbidden. Such regions are called the photonic band gaps (PBGs) analogous to the electronic band gaps (EBGs) in solids. With the existence of PBGs, engineering PBGs to realize certain photonic devices has attracted much attention in the optical and photonic communities. For a simple one-dimensional (1D) PC, a popular application is to design narrowband transmission ﬁlters. Such a ﬁlter Received 1 January 2013, Accepted 19 February 2013, Scheduled 22 February 2013 * Corresponding author: Chien-Jang Wu (jasperwu@ntnu.edu.tw). 360 Liu and Wu with a structure of (LH)N /D/(HL)N or (LH)N /D/(LH)N is referred to as a multilayer Fabry-Perot resonator (FPR) [1]. Filters are used as a wavelength (frequency) selective device which is of particular importance in optical electronics and communications. PC-based optical ﬁlters, which have a feature of tuning, are more practical and interesting to the community in recent years. Depending on the tuning agent, there are several ways to make a ﬁlter tunable. We can make a temperature-tuning ﬁlter by using liquid-crystal as a defect layer [2–4]. Temperature-tunable ﬁlter is also obtainable with a superconducting defect [5–10]. If the defect material is a ferroelectric, then the tuning can be achieved by the external electric ﬁeld (or applied bias voltage) [11]. Filters that are tuned by the magnetic ﬁeld are also available thus far [12, 13]. It should be noted that, in reality, once the crystal is made, there is not variation in the crystal structure in terms of temperature, electric ﬁeld or magnetic ﬁeld as mentioned in the above references. Thus, a ﬁlter with tunable feature can be achieved only by the defect material whose permittivity or permeability is a function of temperature, electric ﬁeld or magnetic ﬁeld. In addition to the above-mentioned tuning, there is another tuning for the narrowband ﬁlter, i.e., use of semiconducting material as a defect layer. For the intrinsic semiconductors, tuning can be made by the variation of intrinsic carrier density which is a strong function of the temperature. For the extrinsic semiconductors, tuning is obtained by changing the doping density. Photonic structures containing extrinsic semiconductors such as n-Si, n-Ge, and n-InSb have been reported recently [14–19]. The purpose of this paper is to investigate the ﬁltering properties for SiO2 /InP photonic crystal containing a defect of n-Si. PC made of SiO2 /InP bilayers has been fabricated and its defective structure for narrowband ﬁlter design is reported recently [20, 21]. This ﬁlter is designed to operate at near infrared (NIR) wavelength. In this work, based on the use of SiO2 /InP-PC, we would like to make a detailed analysis on the ﬁltering properties in a narrowband transmission ﬁlter by adding a defect layer of n-Si. We choose n-Si because it is a strongly dispersive extrinsic semiconductor. Its dielectric function is strongly dependent on the doping density. It will be seen that the position of transmission peak can be changed by the doping density. Thus, by varying the doping density, the proposed structure can be used as an alternative for the design of a tunable ﬁlter called an N -tuning ﬁlter [16]. Our analysis is made by the transmittance which can be calculated by making use of the transfer matrix method (TMM) [22]. The TMM has been widely used in the analysis of electromagnetic wave properties in 1D PCs [23–27]. We shall show how the transmission peak Progress In Electromagnetics Research, Vol. 137, 2013 361 Figure 1. A one-dimensional ﬁlter structure, (LH)N /D/(HL)N , where L = SiO2 , H = InP are the low-, high-index layers, respectively, and the center D = n-Si is the defect layer. The optical wave with a unit power impinges obliquely at z = 0, and R, T represent reﬂectance and transmittance, respectively. (channel wavelength) will be shifted by the variation of doping density, the defect thickness, and the angle of incidence for both TE and TM waves. 2. BASIC EQUATIONS In the analysis that follows, we shall use the calculated transmittance for a one-dimensional defective photonic crystal shown in Figure 1 to study the ﬁltering properties. Here, n-Si is used for the defect layer. Since, the tunable feature arises from the use of n-Si, it is necessary to ﬁrst describe its dielectric function. For an n-Si semiconductor, the dielectric function including the absorption can be described by the plasma model, namely [15] 2 2 ωph ωpe − 2 , (1) εD (ω) = ε∞ 1 − 2 ω − j τωe ω − j τωh where ε∞ is the high-frequency dielectric constant, and τe and τh are the electron and hole scattering times related to the carrier mobilities μe,h by me,h μe,h , (2) τe,h = e where μe,h is expressed as, μe = 92 + 1+ 1268 Nd 1.3×1017 0.91 , μh = 54.3 + 1+ 406.9 Nd 2.35×1017 0.88 , (3) 362 Liu and Wu where Nd is the donor density (in unit of cm−3 ), and the electron and hole plasma frequencies are given by 1/2 ne,he2 ωpe,h = . (4) me,h ε∞ ε0 Here, me is the eﬀective mass of electron and mh is the eﬀective mass of hole which can be determined by the eﬀective masses of the light (mlh ) and heavy (mhh ) holes, 1 + r 3/2 , (5) r + r 3/2 where r = mhh /mlh , ne,h are the densities of electron and hole given by N 2 Nd , (6) ne,h = n2i + d ± 4 2 mh = mhh where ni is the intrinsic density and √ N the donor density. The εD . It is worth mentioning refractive index of n-Si is nD = that the doping-dependent mobilities in Equation (3) are suited at 300 K [28]. These two relationships are accurately empirical and widely applied to compute the carrier mobilities for the doped Si. In addition, Equation (5) arises from the fact that Si is a multiple-valley semiconductor, leading to the diﬀerent eﬀective masses for holes in distinct bands. To analyze the ﬁltering properties, we shall capitalize on the transmittance spectrum for the structure in Figure 1, in which the thicknesses of L, H, and D are denoted by dL , dH , and dD , respectively. The transmittance and reﬂectance can be calculated through the use of the transfer matrix method (TMM) [22]. According to TMM, transmittance T and reﬂectance R are determined by the following expressions, M21 2 1 2 2 2 , , T = |t| = (7) R = |r| = M11 M11 where r and t are the reﬂection coeﬃcient and transmission coeﬃcient, and M11 , M21 are the two matrix elements of the following total system matrix M11 M12 −1 N −1 DD PD DD = D0−1 DL PL DL−1 DH PH DH M21 M22 N −1 DL PL DL−1 D0 . (8) DH PH DH Progress In Electromagnetics Research, Vol. 137, 2013 363 Here, Pi (i = L, H, and D) is the propagation matrix in layer i given by exp (jki di ) 0 Pi = , (9) 0 exp (−jki di ) where ki = ωni /c is the wave number in layer i, and Dq (q = 0, L, H, and D) is the dynamical matrix in medium q which is dependent on the polarization of the incident wave, i.e., 1 1 (TE wave), (10) Dq = nq cos θq −nq cos θq cos θq cos θq (TM wave), (11) Dq = nq −nq where q = 0 is for the air with ε0 = 1. 3. NUMERICAL RESULTS AND DISCUSSION The material parameters for the defect layer, n-Si, in our calculation are ni = 1.5 × 1010 cm−3 , ε∞ = 11.7, me = 0.26m0 , mhh = 0.49m0 , and mlh = 0.16m0 , where m0 = 9.1 × 10−31 kg is the mass of free electron [15]. The low-index dielectric is SiO2 with nL = 1.45 and the high-index one is InP with nH = 3.52 [21]. 3.1. Transmission Peaks as a Function of Thickness in n-Si Let us ﬁrst investigate how the transmission peaks vary as a function of the defect thickness of n-Si. In Figure 2, we plot the transmittance spectrum (blue color) for the ideal PC of (LH)N , where thicknesses Figure 2. Calculated normal-incidence transmittance spectra for ideal PC of (LH)N (blue) and defective PC (red). Here, the thickness of n-Si is dD = 1 mm and the doping density is Nd = 1 × 1017 cm−3 are used in our calculation. 364 Liu and Wu Figure 3. Normal-incidence transmittance spectra for the defective PC with diﬀerent defect thicknesses of dD = 5, 10, 15, 20, 30, 40 µm, respectively. The doping density is ﬁxed at Nd = 1 × 1017 cm−3 . dL = 4.54 µm, dH = 1.22 µm, and N = 20 are used. It can be seen that, at NIR, there is a PBG with left and right band edges at λL = 2.6786 µm and λH = 2.7647 µm, respectively. Our goal is to engineer this PBG to realize a transmission narrowband ﬁlter based on the addition of defect layer. When the n-Si is placed in the middle as a defect layer, there appears a transmission peak (indicated by the arrow) at λp = 2.7272 µm with a peak height of T = 0.9598. Here, the doping density is Nd = 1 × 1017 cm−3 and defect thickness dD = 1 µm are taken. The peak position locates in the vicinity of the gap center of PC of (LH)N . Figure 3 shows how the number of transmission peaks changes as the defect thickness increases. It can be seen that there is a single transmission peak when dD is smaller than 10 mm. At dD = 10 and 15 µm, there are two peaks within the PBG in Figure 2. At dD = 20 and 30 µm, three peaks are generated. As dD is increased up to 40 µm, ﬁve peaks can be obtained. This means that a multichannel ﬁlter can be achieved by increasing the thickness of the defect layer, which is consistent with the result reported by Ghosh et al. [21]. A ﬁlter with multiple channels is of technical use in a wavelength division Progress In Electromagnetics Research, Vol. 137, 2013 365 multiplexing (WDM) application which is of important in optical communications. 3.2. Transmission Peaks as a Function of Doping Density in n-Si We now study the shifting feature in such a ﬁlter structure. The shifting comes from the variation of the doping density in n-Si. With the same thicknesses for SiO2 and InP. In Figure 4, we plot the transmittance spectra at dD = 1 µm for diﬀerent donor densities of Nd = 1×1016 , 1×1017 , 5×1017 , 1×1018 , 3×1018 , and 5×1018 cm−3 . It can be seen that the ﬁltering is changeable since the peak wavelength λp is blue-shifted as the doping density increases. At a density of 1 × 1016 cm−3 , a nearly total transmission can be attained because of near unity peak height. In addition to the blue-shift, the peak shape is also broadened along with a lowering in the peak height. At high density of 5 × 1018 cm−3 , the peak height is greatly suppressed and negligibly small. In order to remain the ﬁltering feature at higher doping density, the thickness dD of n-Si is required to be thinner. This result is illustrated in Figure 5, in which dD has been reduced to 0.1 µm from 1 µm. For thinner defect, the transmission peak is high enough to maintain the ﬁlter requirement even at a highly doped defect of n-Si. In addition, a similar blue-shift in Figure 4 is also seen and the extent of shift is smaller than that in Figure 5. Figure 4. Normal-incidence transmittance spectra for the defective PC with diﬀerent doping densities Nd = 1 × 1016 , 1 × 1017 , 5 × 1017 , 1 × 1018 , 3 × 1018 , and 5 × 1018 cm−3 , respectively. The thickness of n-Si is ﬁxed at dD = 1 µm. 366 Liu and Wu Figure 5. Normal-incidence transmittance spectra for the defective PC with diﬀerent doping densities Nd = 1 × 1018 , 5 × 1018 , 1 × 1019 , and 2 × 1019 cm−3 , respectively. The thickness of n-Si is ﬁxed at dD = 0.1 µm. 3.3. Transmission Peaks as a Function of Angle of Incidence We have so far investigated the ﬁltering properties in the case of normal incidence. We now turn our attention to the angular dependence of ﬁltering for this ﬁlter structure. To investigate the angle-dependent properties, the results of two polarizations, TE and TM, for the incident wave will be given. In Figure 6, transmittance spectra at diﬀerent angels of incidence, θ0 = 0◦ , 5◦ , 10◦ , and 15◦ , respectively, are shown for the TE wave at dD = 0.1 µm and Nd = 1 × 1018 cm−3 . Some features are of note. First, the transmission peak is blue-shifted as the angle increases. The PBG structure also is blue-shifted. And the size of PBG is enhanced when the angle is increased. For TM wave, all these three features are also found and thus are not replotted here. 3.4. Modified Structure for Multichannel Filters The considered structure shown in Figure 1 can be modiﬁed to achieve a multichannel ﬁlter. This can be done by the structure with coupled defects, namely, (LH)N /(LHLD)M LHL/(HL)N [29]. In this structure, multiple channels are generated within the PBG and the channel number is equal to M , the number of coupled defects. Thus, using n-Si as a defect layer of D in this modiﬁed structure, we can make the ﬁlter changeable because the peak positions can be shifted by the variation of doping density. Shifting features are expected to be similar Progress In Electromagnetics Research, Vol. 137, 2013 367 Figure 6. TE-wave transmittance spectra for the defective PC with a doping densities Nd = 1 × 1018 cm−3 and thickness dD = 0.1 µm for diﬀerent angles of incidence, 0◦ , 5◦ , 10◦ , and 15◦ , respectively. to those described previously. Besides, the defect layer D can also be chosen to be other semiconductor like n-Ge or n-InSb such that the shifting in multichannel ﬁlter is achieved. 4. CONCLUSION The ﬁltering properties for a defective PC operating in NIR region have been analyzed in this work. With a defect of n-Si, which is a dispersive and absorptive medium, we have found that the channel wavelength is shown to be blue-shifted when the doping density increases. At a moderate doping density, the ﬁltering can be obtained at a thicker defect layer, whereas a thinner defect is required for a highly doped nSi. In the angular dependence, it is found that the channel wavelength is also blue-shifted as a function of angle of incidence for both TE and TM waves. By increasing the defect thickness, it is possible to obtain a multichannel ﬁlter. A ﬁlter with features of multiple channels and of shifting is of particular use in the optical communications. 368 Liu and Wu ACKNOWLEDGMENT C.-J. Wu acknowledges the ﬁnancial support from the National Science Council of the Republic of China (Taiwan) under Contract No. NSC100-2112-M-003-005-MY3 and from the National Taiwan Normal University under NTNU100-D-01. REFERENCES 1. Orfanidis, S. J., Electromagnetic Waves and Antennas, Rutger University, 2008, www.ece.rutgers.edu/∼orfanidi/ewa. 2. Choudhury, P. K. and W. K. Soon, “TE mode propagation through tapered core liquid crystal optical ﬁbers,” Progress In Electromagnetics Research, Vol. 104, 449–463, 2010. 3. McPhail, D., M. Straub, and M. Gu, “Optical tuning of threedimensional photonic crystals fabricated by femtosecond direct writing,” Applied Physics Letters, Vol. 87, 091117, 2005. 4. Halevi, P., J. A. Reyes-Avendano, and J. A. Reyes-Cervantes, “Electrically tuned phase transition and band structure in a liquidcrystal-inﬁlled photonic crystal,” Physical Review E, Vol. 73, R040701, 2006. 5. Bermann, O. L., Y. E. Lozovik, S. L. Eiderman, and R. D. Coalson, “Superconducting photonic crystals,” Physical Review B, Vol. 74, 092505, 2006. 6. Wu, C.-J., C.-L. Liu, and W.-K. Kuo, “Analysis of thicknessdependent optical properties in a one-dimensional superconducting photonic crystal,” Journal of Electromagnetic Waves and Applications, Vol. 23, Nos. 8–9, 1113–1122, 2009. 7. Lyubchanskii, I. L., N. N. Dadoenkova, A. E. Zabolotin, Y. P. Lee, and Th. Rasing, “A one-dimensional photonic crystal with a superconducting defect layer,” Journal of Optics A: Pure Appl. Opt., Vol. 11, 114014, 2009. 8. Lin, W.-H., C.-J. Wu, T.-J. Yang, and S.-J. Chang, “Terahertz multichanneled ﬁlter in a superconducting photonic crystal,” Optics Express, Vol. 18, 27155–27166, 2010. 9. Anlage, S. M., “The physics and applications of superconducting metamaterials,” Journal of Optics, Vol. 13, 024001, 2011. 10. Hu, C. A., J.-W. Liu, C.-J. Wu, T.-J. Yang, and S.-L. Yang, “Eﬀects of superconducting thin ﬁlm on the defect modes in a heterostructure photonic crystal,” Solid State Communications, Vol. 157, 54–57, 2013. 11. Wu, C.-J., J.-J. Liao, and T. W. Chang, “Tunable multilayer Progress In Electromagnetics Research, Vol. 137, 2013 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 369 Fabry-Perot resonator using electro-optical defect layer,” Journal of Electromagnetic Waves and Applications, Vol. 24, No. 4, 531– 542, 2010. Qi, L.-M. and Z. Yang, “Modiﬁed plane wave method analysis of dielectric plasma photonic crystal,” Progress In Electromagnetics Research, Vol. 91, 319–332, 2009. Tian, H. and J. Zi, “One-dimensional tunable photonic crystals by means of external magnetic ﬁelds,” Optics Communications, Vol. 252, 321–328, 2005. Halevi, P. and F. Ramos-Mendieta, “Tunable photonic crystals with semiconducting constituents,” Physical Review Letters, Vol. 85, 1875–1878, 2000. Halevi, P., A. S. Sanchez, and E. Galindo-Linares, “Tuning and switching of spontaneous emission in one-dimensional photonic crystals,” Optics Communications, Vol. 269, 351–355, 2007. Galindo-Linares, E., P. Halevi, and A. S. Sanchez, “Tuning of one-dimensional Si/SiO2 photonic crystals at the wavelength of 1.54 mm,” Solid State Communications, Vol. 142, 67–70, 2007. King, T.-C., Y.-P. Yang, Y.-S. Liou, and C.-J. Wu, “Tunable defect mode in a semiconductor-dielectric photonic crystal containing extrinsic semiconductor defect,” Solid State Communications, Vol. 152, 2189–2192, 2012. Hung, H.-C., C.-J. Wu, T.-J. Yang, and S.-J. Chang, “Enhancement of near-infrared photonic band gap in a doped semiconductor photonic crystal,” Progress In Electromagnetics Research, Vol. 125, 219–235, 2012. Hung, H.-C., C.-J. Wu, T.-J. Yang, and S.-J. Chang, “Analysis of tunable multiple-ﬁltering property in a photonic crystal containing strongly extrinsic semiconductor,” Journal of Electromagnetic Waves and Applications, Vol. 25, Nos. 14–15, 2089–2099, 2011. Tan, C., G. Fan, T. Zhou, S. Li, and H. Sun, “Preparation of InP-SiO2 3D photonic crystals,” Physica B, Vol. 363, 1–6, 2005. Ghosh, R., K. K. Ghosh, and R. Chakraborty, “Narrow band ﬁlter using 1D periodic structure with defects for DWDW systems,” Optics Communications, Vol. 289, 75–80, 2013. Yeh, P., Optical Waves in Layered Media, John Wiley & Sons, Singapore, 1991. Tolmachev, V. A., A. V. Baldycheva, K. Berwick, and T. S. Perova, “Inﬂuence of ﬂuctuations of the geometrical parameters on the photonic band gaps in one-dimensional photonic crystals,” Progress In Electromagnetics Research, Vol. 126, 285–302, 2012. 370 Liu and Wu 24. Wu, C.-J., T.-J. Yang, C. C. Li, and P. Y. Wu, “Investigation of eﬀective plasma frequencies in one-dimensional plasma photonic crystals,” Progress In Electromagnetics Research, Vol. 126, 521– 538, 2012. 25. Dai, X., Y. Xiang, and S. Wen, “Broad omnidirectional reﬂector in the one-dimensional ternary photonic crystals containing superconductor,” Progress In Electromagnetics Research, Vol. 120, 17–34, 2011. 26. Mouldi, A. and M. Kanzari, “Design of microwave devices exploiting ﬁbonacci and hybrid periodic/ﬁbonacci one dimensional photonic crystals,” Progress In Electromagnetics Research B, Vol. 40, 221–240, 2012. 27. Zhang, H. F., S. Liu, X.-K. Kong, B.-R. Bian, and X. Zhao, “Properties of omnidirectional photonic band gaps in ﬁbonacci quasi-periodic one-dimensional superconductor photonic crystals,” Progress In Electromagnetics Research B, Vol. 40, 415–431, 2012. 28. Pierret, R. F., Semiconductor Device Fundamentals, AddisonWesley, Massachusetts, 1996. 29. Hsu, H.-T., M.-H. Lee, T.-J. Yang, Y.-C. Wang, and C.-J. Wu, “A multichanneled ﬁlter in a photonic crystal containing coupled defects,” Progress In Electromagnetics Research, Vol. 117, 379– 392, 2012.